### Fatigue Crack Growth Fundamentals in Shape Memory Alloys

Y. Wu1•_{A. Ojha}1•_{L. Patriarca}1•_{H. Sehitoglu}1

Published online: 22 April 2015

### Introduction

The shape memory alloys used in engineering and bio-medical applications undergo repeated (cyclic) deforma-tion [1, 2]. These alloys undergo reversible, thermo-elastic phase transformations at the macro-scale, while a degree of irreversibility exists when slip occurs locally at micro-s-cale. The fatigue damage tolerance of these alloys has been a tremendous concern, yet an understanding remains elu-sive as of today. This is partly because our knowledge of fatigue crack growth is built upon untransforming alloys, while the transformation behavior modifies the driving force parameters. In the case of untransforming materials, the stress intensity factor and the crack tip displacements are used to characterize fatigue crack growth. In the case of shape memory alloys, these parameters change but the exact nature of the changes in the driving force that occur has not been derived.

Table 1 illustrates the mechanisms that have been for-warded to modify the driving forces in the presence of phase transformation from austenite to martensite. The modifications in driving force due to internal tractions (first row) have been derived by Rice–McMeeking–Evans [3, 4] using weight function theory. The transformation strains drive these tractions. Also as shown in Table 1 (second row), there have been several efforts attempting to calcu-late the redistribution of stress fields ahead of the crack tip due to the phase transformation. These analyses [5], similar to the work of Irwin on plastic zone size correction [6], propose a change in effective crack length, resulting in a change in the stress intensity factor. A number of recent works on the numerical [7–9] determination of transfor-mation zones under monotonic deformation have been undertaken. The local driving forces are found to differ compared to remotely evaluated levels.

& H. Sehitoglu [email protected]

1 _{Department of Mechanical Science and Engineering,}

University of Illinois at Urbana-Champaign, Urbana, IL 61801, USA

There have been previous fundamental works on fatigue crack initiation in shape memory alloys [10–16] describing the role of slip, the origin of irreversibilities, and residual martensite, but much less work has been undertaken on fatigue crack growth behavior. Systematic efforts have been undertaken by Ritchie and his students [17–19] on experimental fatigue crack growth studies on NiTi alloys. Overall, the measured threshold stress intensity levels were rather low (less than 3 MPapﬃﬃﬃﬃm) in NiTi. Other papers confirmed the low fatigue crack growth resistance of shape memory alloys in general [13, 20, 21]; however, the cal-culation of effective stress intensity in fatigue remains unresolved.

We note that under cycling loading eigenstrains (misfit
strains) arise when transformation develops in the matrix.
Under fatigue conditions both the maximum stress
in-tensity and minimum stress intensity levels are modified
due to the transformation effects. The maximum stress
intensity (Fig. 1a) is reduced as K_{redmax } while the
minimum stress intensity is decreased by Kredminresulting

in a net reduction of the stress intensity range, rendering an effective range denoted as DKeff¼ DK DKred(shaded

region). In this work, we propose a cal-culation methodology for these quantities. The effective stress intensity range would remain the same if the reductions of stress intensity at maximum and minimum loads were identical.

Because we are considering the differential reduction in maximum and minimum stress intensity, the consideration of moduli difference between martensite and austenite domains becomes significant. The martensite under consideration is ‘oriented martensite’ and not the ‘thermally induced martensite’ [22]. The elastic moduli of oriented martensite differ from the thermally induced one and also from the austenite moduli, and this difference cannot be ignored. The martensite crystal moduli tensor (monoclinic or tetragonal depending on the alloys considered here) has higher number of independent constants than the cubic austenite. Also, in this study, our experiments utilize single crystals of austenite permitting precise knowledge of the elastic constants.

In Fig.1b, the main variables that influence the
trans-formation mediated fatigue crack growth rate are listed.
The equivalent eigenstrain, e_{mn}, is calculated from
Eshel-by’s equivalent inclusion principle; the crack length, a;
transformation height in the crack wake, w; the elastic
moduli of the austenite, Cijkl; and martensite, C

0

ijkl, phases

respectively (see Fig.1b). Because the stress state at the crack tip is rather complex, the resulting strain distribution is difficult to predict but it can be measured experimentally. Even though the residual strain per one cycle is very small, it accumulates over many fatigue cycles. The crack length and transformation zone height in the wake can also be obtained through experiments. The elastic moduli can also be measured for the austenite single crystals, while density

Table 1 A summary of the mechanisms at crack tips undergoing transformation under loading Type of

loading-mechanism

Schematic Important variables References

Monotonic loading-shielding associated with tractions

Dimensions of the residual transformation zone in the crack wake, tractions cancel ahead of tip but substantial on crack faces

[3,4]

Monotonic loading-modification of crack tip stress fields

Redistribution of stress fields ahead of crack tip, stress state dependence of transformation zone

[5]

Fatigue loading-closure force differential at max. and min. loads

Elastic moduli (crystallography), transformation zone (verified with DIC), residual transformation strain, reduction of stress intensity range

This study

The tractions due to transformation are shown at the austenite to martensite interface. The differences of closure forces at the minimum and maximum stress intensity levels are important in fatigue case (this study)

the current work, the displacement fields are measured in the vicinity of crack tip during fatigue experiments with digital image correlation (DIC). These displacement results can be utilized in turn to determine the ‘effective stress intensity’ levels. In the case of transforming alloys, these measured displacement fields would naturally reflect the crack tip driving force modification in the presence of transformation strains. As an extension of the method using regression, it is worthwhile to measure the contact of crack surfaces during fatigue resulting in crack closure. Such experiments are now possible with the use of virtual ex-tensometers behind the crack tip in conjunction with digital image correlation studies. We explore this possibility as well in the current work accounting for a full range of mechanisms. The results from regression and virtual ex-tensometers agreed in untransforming alloys, and a similar agreement is expected in shape memory materials. Alter-nately, in the second approach (Method II), we compute the modified stress intensity in transforming alloys due to in-ternal tractions. In fatigue loading, one needs to consider tractions at both maximum and minimum loads imposed on the transforming regions by the surrounding untransformed domains. Ideally, both approaches (I and II) should render an ‘effective stress intensity range’ that is comparable in magnitude resulting in the true value of the driving force in fatigue.

To develop an appreciation of the length scales for the experimental and modeling work pursued in this work, we include Fig.2. At the smallest length scales, atomistic simulations provide a critical resource to establish the elastic constants [22–24] of austenite and martensite which can be substantially different. At the higher length scale, a micro-mechanics analysis is undertaken to determine the closure forces in the wake of the crack tip. Consideration of the theoretical transformation strains and experimentally measured transformation strains are taken into account. The modeling results are verified by precise measurements of crack tip displacements with DIC, and closure stress levels are determined with virtual extensometers at the macro-scale. The paper will cover the entire length scales in Fig. 2with theory and experimentation.

In summary, the driving force for fatigue crack growth in shape memory alloys (the effective stress intensity range) requires additional calculations and depends on the closure forces at both maximum and minimum load, the elastic moduli of austenite and martensite and their anisotropy. The irreversible (residual) strain accumulates with cycles and the residual transformation strain in the crack wake produces closure forces. In turn, such forces contribute significantly to setting an ‘effective stress in-tensity range’ lower than the theoretical one. In the present work utilizing anisotropic elasticity theory, Eshelby’s equivalent inclusion principle [25], weight function

Fig. 1 a The full stress intensity range, the reductions in maximum and minimum stress intensity levels due to transformation induced tractions. The definition of an effective stress intensity range is shown. Note that DKeff ¼ DK DKred ¼ DK ðKredmax KredminÞ.

b Schematic of fatigue crack growing in a shape memory material. The effective stress intensity range is influenced by the residual transformation zone (colored red), the equivalent eigenstrain dictated by the moduli tensors of austenite and martensite, and the internal tractions indicated with arrows. Note that eigenstrain corresponding to maximum and minimum loads are calculated

function theory (DFT) calculations need to be utilized in
the case of martensite. Considering all the factors, we
postulate that the fatigue crack growth rate is given as
a function of C0_{ijkl}, Cijkl, a, w, and e , as da¼

mn dN

f ðDKeffðC

0

ijkl; Cijkl; a; w; eÞÞ. Experimentally, crack tip mn

displacements field measurements can be used to extract stress intensity levels. In the first approach (Method I) of

Then, in ‘‘Method I: Extraction of Stress Intensity Factor from Displacements Using Anisotropic Elasticity via Re-gression’’ section, Method I (regression to extract effective stress intensity range) is described. In ‘‘Method II: Calcu-lation of the Driving Force Changes Due to Transformation Shielding in Crack Wake-Equivalent Eigenstrain Deter-mination-Minimum and Maximum Load’’ section, Method II (modeling to determine effective stress intensity range) is outlined and the results are extended to two other shape memory alloys. The modification in stress intensity ob-tained from Method I and Method II and the experimental fatigue crack growth rates are given in ‘‘Fatigue Crack

Fig. 2 The methodology utilized in the present work. At the atomic scale, the elastic moduli tensor is determined through ab initio calculations, at the micro scale quantities such as transformation strain and the modification of crack driving forces can be calculated.

methods for anisotropic media [26], density functional theory (DFT) calculations, extensive digital image corre-lation results for displacements in crack wake and in transformation zones, we establish the modified stress in-tensity factor for fatigue crack growth in Ni54Fe19Ga27 shape

memory alloy. The elastic moduli and details of the fatigue crack growth experiments are presented in ‘‘Mate-rials, Elastic Moduli and Fatigue Crack Growth Ex-periment Details’’ section. In ‘‘Digital Image Correlation of the Crack Tip Strains in Cyclic Loading’’ section, ex-perimental determinations of strain fields at crack tips ob-tained via DIC and strain irreversibility are demonstrated.

At the macro scale, the stress intensity and the fatigue crack growth on single-crystal specimens are measured through DIC displacement and strain fields at the crack tip, also in the presence of residual strains

Growth Experiments and Corrections to Stress Intensity’’ section. Finally, in ‘‘Virtual Extensometer Results: Deter-mination of Crack Opening Load’’ section, the measure-ments of crack opening and closure loads with virtual extensometers are presented.

### Materials,

### Elastic Moduli, and Fatigue Crack

### Growth

### Experiment Details

Material

The material studied experimentally in this study is
Ni54Fe19Ga27(hereafter referred to as Ni2FeGa for the sake
of simplicity) which undergoes cubic to tetragonal
trans-formation (Fig. 3). It is a new class of shape memory alloys
which exhibits multi-martensites with strain levels
ex-ceeding 10 % [27–29]. The materials undergoes L2_{1 }to
10 M to 14 M to L1_{0 }tetragonal transformation. The typical
stress–strain response for Ni2FeGa is summarized in

Fig. 4a and b for deformation in tension. Figure 4a shows orientation dependence and the modulus difference among the three crystallographic orientations analyzed in this study. Figure 4b shows the two-stage transformation and transformation strain levels exceeding 10 %. More details are provided in Appendix 4.

Based on the lattice deformation theory calculations [30], the maximum transformation strains are known for all three orientations. Among the three orientations considered in this study, the [001] strain is as high as 12 %, while the [011] strain is 3.5 %, and the [123] strain is 4.5 %. The magnitude of the residual or accumulated strain is a frac-tion of the maximum strain, and based on careful mea-surements, we measured this strain as slightly less than 0.8 %.

The elastic moduli tensors for austenite and tetragonal martensite phases need to be known for the calculations. The austenite constants can be determined experimentally

and are given in Table 4 (also graphically plotted in Fig. 5a), but the martensite elastic constants need to be evaluated from atomistic simulations. DFT calculations were made for the martensitic state (L10).

DFT Simulation Setup

In order to calculate the elastic constants of martensitic Ni2FeGa, a cell structure consisting a total of 8 atoms was used. The cell consisted of four Ni, two Fe and two Ga atoms, thus maintaining an atomic ratio of Ni, Fe, and Ga as 2:1:1. We employed first principles calculations based on the DFT to obtain the total-energy of the system. We utilized the Vienna ab initio simulations package (VASP) with the projector augmented wave (PAW) method and the generalized gradient approximation (GGA) as implemen-tations of DFT [31]. In our calculations, we used a 12 9 12 9 12 Monkhorst–Pack k-point meshes for the Brillouion-zone integration to ensure the convergence of results. The energy cut-off of 500 eV was used with the plane-wave basis set and a conjugate gradient algorithm was performed for ionic relaxation ensuring an energy convergence to less than 5 103 eV/A˚ .

To calculate the elastic constants of the martensitic (L10 -non-modulated Ni2FeGa), we obtained the total en-ergy variation of the crystal as a function of the volume subjected to six different distortions (strain). The defor-mation tensors given in Voigt notation and the corre-sponding energy densities are given in Table 2. The strain parameter d in Table 2 for each deformation was varied from -0.03 to 0.03 in the present analysis. After obtaining the total energies E and E0 for the strained and the un-strained lattice

respectively, the parameter ðE E0Þ=V0values were then

plotted as a function of strain (e), where V0 is the

equilibrium volume. The elastic constants were then extracted from the second-order coefficient fit of the following equation:

Fig. 3 The crystal lattices of cubic austenite (L21) and tetragonal martensite (L10). The lattice constants are established with DFT calculations which are then in turn used for determination of the elastic moduli tensors

Fig. 4 aStress–strain response of Ni2FeGa in tension for three orientations considered in this study, b stress–strain response to high strains for

the [001] case in tension. Note that the maximum transformation strains are rather high as high as 12 % in this material

Fig. 5 Elastic moduli of Ni2FeGa, a Austenite modulus

as a function of crystal orientation, b Martensite modulus tensor, the difference in [001] and [010] represent ‘‘c’’ and ‘‘a’’ axis, respectively

E V;ð eÞ ¼ E Vð 0; 0Þ þ V0 X6 i¼1 rieiþ V0 2 X6 i;j¼1 Cijeiejþ O d3 ;

Table 2 Distortion matrices and energy densities for elastic constant calculations of martensitic Ni2FeGa

Structure Distortion matrix DE=Vo

Martensite (L10) _{e}_{1}_{¼ d}2_{=ð1 d}2_{Þ; e}
4¼ d 2C44d2þ Oðd4Þ
e3¼ d2=ð1 d2Þ; e6¼ d 2C66d2þ Oðd4Þ
e1¼ d; e2¼ d; e3¼ d2=ð1 d2Þ ðC11 C12Þd2þ Oðd4Þ
e1¼ d; e2¼ d2=ð1 d2Þ; e3¼ d 1=2 Cð 11 2C13þ C33Þd2þ Oðd4Þ
e1¼ e2¼ e3¼ d ðC11þ C12þ 2C13þ C33=2Þd2þ Oðd4Þ
e3¼ d ðC33=2Þd2þ Oðd4Þ

Table 3 Elastic constants (in GPa) and the corresponding crystal structures of alloys Ni2FeGa, NiTi, and CuZnAl in

martensitic phase

Alloys Crystal structure C11 C22 C33 C44 C55 C66 C12

Ni2FeGa* L10 256 241 212 109 109 45 103

NiTi B190 209 234 238 77 23 72 114

CuZnAl 18R 175 156 235 54 28 48 118

Alloys Crystal structure C13 C15 C23 C25 C35 C46 AM

Ni2FeGa* L10 155 0 155 0 0 0 1.75

NiTi B190 _{102} _{1} _{139} _{-7} _{27} _{-5} _{2.5}

CuZnAl 18R 40 10 150 0 0 -10 16

The data for Ni2FeGa (marked with *) are obtained using DFT in the present analysis. The NiTi and

CuZnAl data are obtained from [22, 32], respectively. The anisotropic ratios (AM) are also given. Note the

very high anisotropy ratio for CuZnAl

Table 4 Elastic constants (in GPa) and the corresponding crystal structure of alloys in austenitic phase noted in the present study Alloys Crystal structure C11 C12 C44 AA

Ni2FeGa L21 163 136 86 5.4

NiTi B2 175 130 31 1.37

CuZnAl B2 116 102 84 12

The data are obtained from [24, 33, 36, 37] respectively. The anisotropic ratios (AA) for three alloys are also given

Fatigue Crack Growth Experiments

Fatigue crack growth experiments were conducted on the Ni2FeGa single crystals for three-crystal orientations:[001],

[123], and [011]. The tensile dog-bone-shaped spe-cimens utilized in this study were cut using EDM and have nominal 1.50-mm 9 3-mm-gage section, 10-mm-gage length and a 0.5-mm notch. Prior to testing, the specimens were polished using SiC paper (from P800 to P1500). Successively, a fine speckle pattern adapted for image correlation was deposited using an Iwata micron B airbrush and black paint. Three experiments were conducted separately on the single crystals. The fatigue crack growth experiment on [001] Ni54Fe19Ga27 was conducted under MTS Landmark Servo

Hydraulic Load Frame to capture the relationship between stress intensity factor range and crack growth rate. For the other two orientations, [011] and [123], two experimental set-ups were prepared. (i) Under

ð1Þ where Cij, ri, ei are the elastic constants, stress, and strain

in Voigt notation. The results are shown in Fig. 5, and the modulus tensor for martensite is provided in Table 3. The total energies to obtain Cð 33=2Þd2þ Oðd4Þ are discussed in

Appendix 5.

In addition to the elastic moduli of martensites, the anisotropy factor is included in the Table 3. The results for NiTi and CuZnAl, two well-known studied alloys in terms of fatigue resistance, are also included in Table 3. The plots of the elastic moduli for NiTi and CuZnAl are given in Appendix 3. The NiTi results are obtained from [22] and the CuZnAl constants are obtained from [32]. The elastic constants for the three materials in the austenitic state are listed in Table 4. The anisotropy factor is also included in Table 4. The procedure for calculating the anisotropy ratio can be found in the work Ostoja-Starzewski [34]. It is important to note that these set of constants meet the me-chanical stability criteria for the elastic moduli. We note that the moduli values for both austenite and martensite are strongly orientation dependent. This information is of fundamental importance for precise calculation of the in-ternal forces acting on the crack surfaces and for deter-mination of the stress intensity levels when displacements are measured.

image correlation results. An example of the strains in the crack wake is shown in Figs. 7 and 8. In Fig. 7, the axial strain fields at the beginning of the cycle (point A) and at the end of the cycle (point B) are shown for the [011] crystal orientation. The strain maps were obtained adopting two image resolutions. Utilizing the 0.44 lm/px set-up the full-field strain field of the notch region can be analyzed, and the extent of the crack wake can be readily obtained. Images captured at higher resolutions (0.22 lm/px for the example reported) are then necessary in order to characterize the crack-tip strain field. From the high-resolution strain fields marked as A and B in Fig. 7, it is possible to calculate the accumulation of the local strains in front of the crack tip following the fatigue cycle.

Providing these strain measurements for different crack lengths, in Fig. 8, we report the strain accumulation during crack propagation in terms of the equivalent strain at the crack tip. The equivalent strain at the crack tip was calculated via averaging the strain tensor components over a region of approximately 50 lm 9 50 lm in front of the crack tip for different crack lengths. That is, within this confined region ahead of the crack tip, the strain components, exx, eyy, and exy, can be extracted from digital image correlation results. Consequently, the corresponding equivalent strain, eEquivalent, can be calculated from Eq. (2). The difference between levels of strain at point A and point B, in Fig. 8, yields the equivalent strain accumulation in one fatigue cycle

eEquivalent¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 3 e 2 xxþ 2e2xyþ e2yy r : ð2Þ

A comparison of the strain fields at peak and minimum load for the three crystal orientations [001], [123], and [011] is illustrated in Fig. 9. The shapes of the transfor-mation region determined using these strain fields will be used to evaluate the reduction in stress intensity factor for each orientation.

### Stress

### Intensity Determination via Regression and

### Modeling,

### Fatigue Crack Growth Rates, Virtual

### Extensometers,

### and Key Variables

### for

### Modeling

Method I: Extraction of Stress Intensity Factor from Displacements Using Anisotropic Elasticity via Regression

The displacement fields from the digital image correlation are shown in Fig. 10. In Figs. 10a and b, the displacements normal and parallel to the crack tip are shown respectively for fatigue crack growth in [001] oriented specimens. These results are fitted to the anisotropic displacement fields for cubic crystals. Such solutions are available by Sih

Fig. 6 The SEM tester that is utilized with high resolution micro-scope to measure the local crack tip displacements for fatigue experiments

the same servo hydraulic load frame, we initially pre-cracked the specimens utilizing constant amplitude load-ings in order to induce a fatigue crack from the notch. For this experimental configuration, the images used for crack length measurements and displacements (in x and y direc-tions) and strain fields correlations were captured using an IMI model IMB-202 FT CCD camera (1600 9 1200 pixel) with a Navitar optical lens, providing an average resolution of approximately 2 lm/px [35]. (ii) Successively, the cracked specimens were loaded under a 4.5 kN EBSD SEMTester which was herein fitted under an Olympus BX51M microscope (Olympus lens). This set-up is shown in Fig. 6 and was utilized for obtaining images at higher magnifications (from 0.44 up to 0.22 lm/px). This set-up allows precisely obtaining the strains at crack tip and the extent of the residual transformation zone. For these three experiments, initial images of the virgin specimens were captured prior to loading (reference images) in order to calculate the accumulated strain in the further analyses.

### Digital

### Image Correlation of the Crack Tip Strains

### in

### Cyclic Loading

Displacement and strain fields were monitored in the vicinity of the crack as the crack advances. These measurements were made at maximum load, minimum load, and at intermediate loads. As the crack advances into a zone of transformed material is generated in the wake of the crack. This zone height and the strains are readily measured from the digital

extracted. In the case of [123] and [011]-oriented single crystals, the crack grew nearly normal to the loading axis and the Mode II stress intensity is small. The crack tip displacements for the [123]-oriented specimens are shown in Fig. 10c. Figures 10a–c demonstrate the comparison between experimental and regression displacement fields.

Fig. 7 Residual strain accumulation during cycling loading of Ni2FeGa oriented

along the [011] crystal direction; the DIC images are taken at minimum load at the beginning of the cycle (point A) and at the conclusion of the cycle (point B) and correlated with the reference image

Fig. 8 The measured accumulation of equivalent strains over a wide range of crack lengths. The accumulated strain per cycle is the difference between the strain levels at points B and A shown in the schematic

et al. [26]. It is possible to extract the stress intensity by regression fit to the following set of equations, Eqs. (3) and (4). We note that the equations include the elastic constants and T stress term. We also note that the orientation of the crack in the [001] specimen is 45° to the loading axis. In this case, both Mode I and Mode II stress intensities can be

A video was attached to this paper to illustrate such com-parison during one fatigue cycle.

The stress intensity factors, K1and K2, can be extracted from horizontal and vertical displacements, u1 and v1, through the following equations

u1¼ K1 ﬃﬃﬃﬃﬃ 2r p Re 1 l1 l2 l1p2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cos hþ l2sin h p l2p1 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cos hþ l2sin h p i þ K2 ﬃﬃﬃﬃﬃ 2r p Re 1 l1 l2 p2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cos hþ l2sin h p p1 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cos hþ l2sin h p þ a11Tr cos hþ Ar sin h þ Bu ð3Þ v1¼ K1 ﬃﬃﬃﬃﬃ 2r p Re 1 l1 l2 l1q2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cos hþ l2sin h p l2q1 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cos hþ l2sin h p i þ K2 ﬃﬃﬃﬃﬃ 2r p Re 1 l1 l2 q2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cos hþ l2sin h p q1 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cos hþ l2sin h p i þ a12Tr cos hþ Ar sin h þ Bv ð4Þ a11l4 2a16l3þ 2að 12þ a66Þl2 2a26lþ a22 ¼ 0; ð5Þ

where Re represents the real part of a complex number, T is the T-stress, A is the rigid body rotation, Buand Bvare the

Fig. 9 The strain fields at the peak and at the minimum loads obtained from fatigue crack growth experiments on Ni2FeGa

utilizing digital image correlation. The results for fatigue loading in three orientations are displayed: [001], [123], and [011]

rigid body translations in u1 and v1 directions, respectively,
a11, a12, a16, a22, a26, and a66 are the compliance
compo-nents, r and h are the polar coordinates with their origin at
the crack tip, and l_{1 }and l_{2 }are the roots of Eq. (5). The p_{i }
and q_{j }in Eqs. (3) and (4) are the anisotropic terms defined in
the following ways

pi¼ a11l2i þ a12 a16li qj¼ a12ljþ a22 lj a26: ð6Þ

Method II: Calculation of the Driving Force Changes Due to Transformation Shielding in Crack Wake-Equivalent Eigenstrain Determination-Minimum and Maximum Load

The strain level measured via DIC is shown in Fig. 9for different single-crystal orientations. Since the transformed area is surrounded by the matrix material, the DIC result can be interpreted as the total strain, et

mnwhich is the sum

of constrained strain and far field strain. The intrinsic

Fig. 10 The crack tip displacements. a Normal to the crack plane (indicated as vertical displacements v), and bhorizontal to the crack plane (horizontal displacements u) for the inclined crack in a single-crystal oriented in [001] orientation. c The vertical crack tip displacements for the single crystal oriented in [123] orientation

transformation strain, ep_{kl} can be calculated by following
equation
ep_{kl}¼ S1
klmn e
t
mn e
o
mn
; ð7Þ

where eo_{mn} is the far-field strain and Sijkl the Eshelby’s

tensor for cubic crystal material. The Sijkl represents the

geometry of the martensite platelets and is treated as a flat ellipsoidal shape. It can be obtained as

Sijkl¼ 1 8pCpqkl Gipjqþ Gjpiq ; ð8Þ

where the specific terms, Gipjq, are given a book by Mura

[38] and also in Appendix 1 for completeness.

Assuming the minimum load to be near zero, the misfit
strain due to modulus mismatch can be neglected. As a
result, in the case of minimum load, ep_{kl} is the equivalent
eigenstrain that needs to be calculated. Therefore, the
corresponding stress, Tij, on the transformation contour can
be obtained via

Tij¼ Cijkle p

kl: ð9Þ

When the maximum load is applied, the eigenstrain
ef-fect due to modulus mismatch, e_{mn}needs to be taken into
account. The equivalent eigenstrain, e_{mn}, which is the sum
of e_{mn} and ep_{kl} can be calculated through Eshelby’s
equivalent method described below

Cijkl e0klþ Sklmnemn e
kl
¼ C_{ijkl}0 e0_{kl}þ Sklmnemn e
p
kl
e_{mn}¼ Cijkl C
0
ijkl
Sklmn Cijmn
h i1
Cijkl C
0
ijkl
e0_{kl} Cijklepkl
h i
; ð10Þ

where C_{ijkl } and C_{ijkl }0 are the elastic moduli of cubic
austenite and tetragonal martensite for Ni2FeGa,
respec-tively. These tensors are given in ‘‘DFT Simulation Setup’’
section. We note that all tensors are given in the cubic
coordinate frame, and the rotations associated with the
transformation are accounted for when the moduli are
determined.

Upon calculation of the equivalent eigenstrains, the corresponding stress, Tij, in the transformation zone can be ascertained as

Tij¼ Cijklekl ð11Þ

Using equation above, it is possible to determine the in-ternal tractions along the transformation contour using the Cauchy formula. Further details are given in Appendix 1.

Knowing the tractions on the surface of transformation zone, we can numerically calculate the stress intensity change for a specific loading case. By implementing the weight function technique proposed by Bueckner and Rice [4], the stress intensity factor due to the internal tractions, DKI, can be written as

DKI ¼

Z

Sp

niTijhjdSp; ð12Þ

where n_{i }is the outward normal of the transformation zone,
dSp is the line element on the perimeter of the zone, and hj
is the anisotropic weight function which is going to be
determined.

According to Rice, the weight function can be readily
obtained through Eq. (13) if the displacement fields, u1 and
v1, and stress intensity factor, K_{1 }and K2, in a reference load
system are known

hx¼ H 2K1 ou1 ol hy¼ H 2K1 ov1 ol : ð13Þ

The solution for stress intensity factors due to tractions on the crack surface in Fig. 11 can be found via Eq. (14) and displacement fields are provided by Sih et al. [26] as

K1¼
1
ppﬃﬃﬃa
Za
0
r xð Þ
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
aþ x
a x
r
1
2
ao
bo
" #
dx
K2¼
1
ppﬃﬃﬃa
Za
0
r xð Þ a
2
o
2b_{o}þ
1
2b_{o}
a12
a11
þ a2
oþ b
2
o
dx;
ð14Þ
where ao and bo are the real and imaginary component of
the roots for Eq. (5), i.e., for l_{1} ¼ ao þ boi and

l_{2 }¼ aoþ boi.

The elastic moduli, H, can be represented in Eq. (15) H¼ 1 8 l1 l2 l2 i aobo a12 a11 þ a2 o b 2 o þ 1 : ð15Þ

Fig. 11 Schematic of the load system on the crack surface. Four zones are considered and the contributions of all four zones are taken into account. Zones 1, 3 and 4 have the most significant influence on the results of stress intensity due to internal tractions

Once weight functions are obtained, the corresponding stress intensity factor in that loading system can be deter-mined through Eq. (13). The summation of stress intensity factors obtained from different parts of the transformation contour (Fig. 11) yields the change of stress intensity factor due to transformation effect. Further details are given in Appendix 2.

The net reduction in stress intensity factor as the applied loading is increased is given in Table 5. The contributions from different sectors of the transformation zone are pro-vided. It is noted that the Zone 2 provides negligible contribution while Zones 1 and 3 provide a smaller con-tribution compared to Zone 4. These results are further presented in the next section.

Fatigue Crack Growth Experiments and Corrections to Stress Intensity

The experimental fatigue crack growth rate results and predictions of fatigue crack growth rates upon correction of stress in intensity range are shown in Fig. 12. The effective stress intensity range upon regression of the entire dis-placement field is also included in Fig. 12. The agreement for the theory and regression-based stress intensity range is excellent. The reduction in the stress intensity range is approximately 35 % of the full range based on regression and also based on theory. We show virtual extensometer results of crack opening displacements confirming the crack closure in the next section.

Virtual Extensometer Results: Determination of Crack Opening Load

The virtual extensometer method is another technique for determining the crack closure levels which is complimen-tary to ‘regression.’ The technique is illustrated in Fig. 13a. The relative displacements across the crack faces are measured during loading and unloading. Therefore, DIC measurements allow the determination of the crack open-ing displacements during loading and unloading. By making such measurements over fine increments, it is possible to precisely determine the applied load level at

which the crack opening occurs. These results are shown in Fig. 13b for two crack lengths. The crack opening load is determined as 35 % of the maximum load.

Sensitivity of Results to a=w Ratio and the Moduli Levels

Three other shape memory alloys were assessed to evaluate the propensity of K reduction. The results are shown in Tables 6 and 7. In the first set of simulations (Table 6), the a=w ratio was maintained at 2. In Table 7, we consider the reductions in K at both maximum and minimum loads for different a=w ratios. A noteworthy point is that the re-duction in K occurs at both maximum and minimum load. However, since the reduction is higher at the maximum load, this results in a net decrease in stress intensity range.

The sensitivity of the simulations on the variations in the a=w ratio and martensite moduli magnitude is studied in Fig. 14a and b. The basis for these simulations is the Ni 2-FeGa alloy. We note that as the a=w ratio increases, with all other parameters constant, the reduction in both mini-mum and maximum stress intensity is noted. The overall reduction in stress intensity range saturates with increasing a=w ratio. In Fig. 14b, the martensite modulus is pre-multiplied by a factor. The factor F = 1 corresponds to the Ni2FeGa case. As the factor increases the reduction in

stress intensity range increases.

### Discussion

### of Results

Fatigue crack growth experiments were conducted on the new Ni2FeGa shape memory alloy. Extensive experimental results and measurements for fatigue crack growth were obtained in the course of this study. Three single-crystal orientations of Ni2FeGa shape memory alloy were tested in

tension–tension fatigue. The experimental results were obtained at room temperature where the material deforms under ‘pseudoelastic’ conditions. The crack advance was measured as a function of the effective stress intensity range and the threshold stress intensity range was precisely established as 8:3 MPapﬃﬃﬃﬃm.

Table 5 Stress intensity factor (KðMPapﬃﬃﬃﬃmÞ) values due to tractions on different zone boundaries of Ni2FeGa in

Fig. 11for the a=w = 2 case

Zone # Zone 1 Zone 2 Zone3 Zone 4 Total

Load (MPa) K1 K2 K3 K4 Kred¼PKi MPa ﬃﬃﬃﬃm

p ð Þ 3.34 0.35 0.013 0.35 -3.07 -2.37 10 0.42 0.018 0.42 -3.69 -2.85 20 0.63 0.023 0.63 -4.75 -3.49 30 0.93 0.028 0.93 -7.03 -5.17 40 1.16 0.033 1.16 -8.75 -6.43 50 1.46 0.039 1.46 -10.9 -7.98

Reduction in stress intensity range (of the order of 30 %) was established by calculating the closure forces (Method II —‘‘Method II: Calculation of the Driving Force Changes Due to Transformation Shielding in Crack Wake-Equivalent Eigenstrain Determination-Minimum and Maximum Load’’ section) via a micro-mechanical analysis. The closure forces arise due to residual strains in the wake of the crack. The calculated crack tip stress intensity range is in agreement with the experimental measurements of the effective stress intensity range. We used two experimental measurements for measuring the effective stress intensity range. In the first one, the crack tip displacement fields were utilized to establish the stress intensity range with a least square fitting procedure (Method I—‘‘Method I: Ex-traction of Stress Intensity Factor from Displacements Using Anisotropic Elasticity via Regression’’ section). This method resulted in establishment of the effective stress intensity range 30 % smaller than the theoretical one. The difference is attributed to shielding due to residual dis-placements in the crack wake. In the second one, by using virtual extensometers along the crack faces (‘‘Virtual Ex-tensometer Results: Determination of Crack Opening Load’’ section), the crack opening and crack closure loads were measured and found to be also at nearly 30 % of the maximum load.

A combined experimental-theoretical methodology is outlined for a better understanding of the driving force for fatigue crack growth in shape memory alloys. The choice

of single crystals allowed precise knowledge of the elastic moduli in the austenitic and martensitic phases. In turn, the moduli tensors were used in a micro-mechanical analysis to determine the equivalent eigenstrains in the transformed regions. The equivalent eigenstrain was used to determine the internal tractions at maximum load of the cycle. This led to the calculation of the reduction in stress intensity, hence a modified range of stress intensity was determined. The calculations presented represent an advancement by accounting for elastic moduli difference and with the ex-perimental determination of strain fields at minimum and maximum loads.

To put perspective on the results, the simulations were repeated on two well-known shape memory materials, the NiTi and CuZnAl. The reductions in stress intensity range were lower in NiTi compared to Ni2FeGa, while the re-duction in CuZnAl was substantially lower than NiTi and Ni2FeGa. These results cannot be directly compared with experiments in the literature, since there is no reported CuZnAl fatigue crack growth data to our knowledge. The literature on NiTi shows threshold levels that are lower compared to Ni2FeGa.

Fatigue crack growth behavior in shape memory alloys remains a complex topic. The elastic moduli evolves con-tinuously; it is strongly orientation dependent in both austenite and martensite. The moduli tensors decide the equivalent eigenstrains, hence the closure forces. The clo-sure forces vary as a function of cycles accompanying the

Fig. 12 Fatigue crack growth behavior of primarily based on experiments on [001] single crystals. The range in effective stress intensity is obtained by regression analysis of crack tip displacements (present experiments) and also via calculation of the shielding effects due to transformation (present theory). The effective threshold stress intensity range is 8.3 MPapﬃﬃﬃﬃm. The full range of stress intensity is also provided as a reference. The dashed lines are drawn to aid the eye

Fig. 13 aSchematic of the virtual extensometer methodology used for crack closure measurements. b The crack opening displacement profiles, utilizing virtual extensometers, for the specimen oriented in [001] direction. The gage location is the distance behind the crack tip. The profiles are given as a fraction of the maximum applied load. The crack opening load is determined as 35 % of the maximum applied load

residual transformation strains. In this study, we estab-lished the modification in stress intensity and established a rigorous estimate of the stress intensity range. In future studies, the crack growth rate needs to be predicted based on the magnitude of the irreversibility in displacements at crack tips [39, 40]. This would require knowledge of the slip and transformation energy barriers in the material [41]. This approach would need to be taken with care because both transformation and plasticity can occur simultane-ously at the crack tips. In the present calculations no ex-plicit consideration of plastic slip was included [41]. Plasticity can occur at high stress levels and it needs to be considered in future work.

Finally, we comment on the role of martensite to austenite modulus change. Evidence of higher martensite modulus relative to austenite is well documented [42]. On the other hand, the martensite modulus is taken as less than the austenite modulus in most constitutive models. The martensite moduli upon deformation in fatigue and fracture studies are the oriented martensite and not the self-acco-modated one [22]. Also, the constitutive models utilized have been simple for the ease of implementation in FEM codes. This creates some difficulty when residual strain buildup due to residual martensite or plastic deformation needs to be considered. There is no provision for these

mechanisms in most constitutive models. Finally, there is the matter of orientation dependence. A highly anisotropic material cannot be represented accurately as isotropic with two elastic constants. Constitutive models will need to incorporate these characteristics.

### Conclusions

The work supports the following conclusions:

(1) The new shape memory alloy Ni2FeGa displays unusually high fatigue thresholds (8:3 MPapﬃﬃﬃﬃm) and excellent fatigue crack growth resistance. The

0.5 1.0 1.5 2.0
0
2
4
6
8 Load
t
**K****max **
**K****min **
*a/w*
0.4 0.6 0.8 1.0 1.2 1.4 1.6
0
2
4
6
8
10
12
Load
t

Martensite Modulus Factor (* F.C'ijkl*)

**K****max **

**K****min **

**(a)**

**(b)**

Fig. 14 a Reduction in maximum and minimum stress intensity levels with increase in crack length, the results are for the [001] Ni2FeGa material and explore the hypothetical variation of residual

transformation zone on the results. b Reduction in maximum and minimum stress intensity levels as a function of martensite modulus factor. The moduli tensor is simply scaled by the factor, F. The F = 1 case corresponds to the baseline Ni2FeGa material

Table 6 The DKredðMPa ﬃﬃﬃﬃm

p

Þ values for alloys noted in the present study

Alloys a=w DKredðMPa ﬃﬃﬃﬃm

p Þ

Ni2FeGa 2 -5.61

NiTi 2 -2.38

CuZnAl 2 -1.91

Table 7 Reduction in stress intensity factor (KredðMPa ﬃﬃﬃﬃm

p

Þ) values for alloys noted in the present study at minimum and maximum loads Alloys a=w Kredmin KredmaxðMPa ﬃﬃﬃﬃm

p Þ Minimum load Maximum load

NiTi 0.5 -1.05 -2.59 1 -1.47 -3.37 2 -1.8 -4.18 4 -2.25 -4.54 Ni2FeGa 0.5 -1.26 -3.06 1 -1.89 -6.74 2 -2.59 -7.34 4 -3.17 -7.77 CuZnAl 0.5 -1.48 -2.81 1 -1.86 -3.5 2 -2.29 -4.2 4 -2.62 -4.7

reduction of the stress intensity range associated with the transformation is considerable as shown with an anisotropic micro-mechanics calculation. (2) Excellent quantitative correlation is achieved between

theory and the experimental measurements of stress intensity range reduction. Utilizing crack tip displace-ment fields with digital image correlation methods allowed evaluation of the effective stress intensity range in agreement with the virtual extensometers along the crack flanks. These results show that the reduction in stress intensity is 35 % of the full range. (3) Comparisons were made between three shape memory alloys to assess their propensity for shielding associ-ated with phase transformations. It was found that the Ni2FeGa produced higher levels of stress intensity reduction compared to NiTi and CuZnAl alloys. The work underscored the role of elastic moduli in the martensitic and austenitic phases on the calculations of the reduction in stress intensity range.

Acknowledgments The work was supported by Nyquist Chair funds at University of Illinois. The authors acknowledge the assis-tance of Mr. George Li.

### Appendix

### 1: Eshelby Tensor for Anisotropic

### Media

The treatment follows that given by Mura [38]. The Eshelby’s tensor calculation is introduced in Eq. (8) Sijkl¼ 1 8pCpqkl Gipjqþ Gjpiq : Gipjq is

For the case of cubic material, the definition of
presented in Eq. (16)
G1111¼ G2222¼
2p
a
Z1
0
1x2
ð Þ
pq 1x
2_{þq}2_{x}2
l
2_{ð1x}2_{þq}2_{x}2_{Þþbq}2_{x}2_{dx}
þp
a
Z1
0
1x2
ð Þ2
p pþqð Þ b 1x
2_{þq}2_{x}2
þcq2_{x}2
dx
G3333¼
4p
a
Z1
0
q2_{x}2
pq 1x
2_{þq}2_{x}2
l2ð1x2_{þq}2_{x}2_{Þ}
þb 1x 2_{dxþ}pc
a
Z1
0
q2_{x}2_{ð}_{1}_{x}2_{Þ}2
p pþqð Þ dx
G1122¼ G2211¼
2p
a
Z1
0
1x2
ð Þ
pq 1x
2_{þq}2_{x}2
l2ð1x2_{þq}2_{x}2_{Þþbq}2_{x}2
þ 1x 2
b 1x 2_{þq}2_{x}2_{þcq}2_{x}2
dx
p
a
Z1
0
1x2
ð Þ2
p pþqð Þ b 1x
2
þq2x2
þcq2x2
dx G1133¼ G2233
¼2p
a
Z1
0
q2_{x}2
pq 2 1x
2_{þq}2_{x}2
l2ð1x2_{þq}2_{x}2_{Þþbq}2_{x}2
þ 1x 2
b 1x 2_{þq}2_{x}2_{þcq}2_{x}2
dx G1212
¼ p kþlð Þ
a
Z1
0
1x2
ð Þ2
p pþqð Þ l 1x
2
þq2x2
þl0q2x2
dx
ð16Þ
G1313¼ G2323
¼ 2pl kð þ lÞ
a
Z1
0
q2_{x}2_{ð}_{1}_{ x}2_{Þ 1 x}_{ð} 2_{þ q}2_{x}2_{Þ}
pq dx
pl
0_{ð}_{k}_{þ l}_{Þ}
a
Z1
0
q2_{x}2_{ð}_{1}_{ x}2_{Þ}2
p pð þ qÞ dx
G3311¼ G3322
¼2p
a
Z1
0
1 x2
ð Þ
pq 1 x
2_{þ q}2_{x}2
l2_{ð1 x}2_{þ q}2_{x}2_{Þ}
þb 1 x 2_{dx} _{þ}pc
2a
Z1
0
1 x2
ð Þ3
p pð þ qÞdx:

Specific terms in Eq. (16) can be represented as the
following,
q ¼ a1=a3
a ¼ l2ðk þ 2l þ l0Þ
b ¼ a1ll0ð2k þ 2l þ l0Þ
c ¼ a1l02ð3k þ 3l þ l0Þ
b ¼ l k þ l þ lð 0Þ
c ¼ l0 ð2k þ 2l þ l0Þ
p¼n1 x2_{þ q}2_{x}23_{þ bq}2_{x}2_{1}_{ x}2_{1}_{ x}2_{þ q}2_{x}2
þ1
4 1 x
2
2
b 1 x2_{þ q}2_{x}2_{þ cq}2_{x}2
1
2
; 0\x\1
q¼n1 x2_{þ q}2_{x}23_{þbq}2_{x}2_{1}_{ x}2_{1}_{ x}2_{þ q}2_{x}2o
1
2
;
0\x\1;
ð17Þ

hx¼ H 2K1 ou1 ol hy¼ H 2K1 ov1 ol ð18Þ

Horizontal displacement u1 and vertical displacement v1
can be found earlier. The stress intensity factor K_{1 }is
pre-sented earlier as well as the elastic modulus H. A schematic
showing a point load with a distance r and oriented at an
angle of h from the crack tip is presented in Fig. 16.

The weight function can be calculated as follows:

hx¼ H 2K1 ou1 oh sin h r ou1 or cos h hy¼ H 2K1 ov1 oh sin h r ov1 or cos h : ð19Þ

### Appendix

### 3: 3D Elastic Moduli Representation

The elastic moduli tensor is represented with 3D images in Fig. 5 for Ni2FeGa. For completeness, we provide the moduli images for the two other alloys, NiTi and CuZnAl (Fig. 17).

### Appendix

### 4: Transformation Strains

The lattice constants of three of the alloys considered result in the following transformation matrix which can be used to establish the transformation strains (Table 8).

The following equation can be used to establish the
transformation strains, e¼pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ^eT_{F}T_{F ^}_{e}_{ 1 where F is the}

deformation gradient and is related to the transformation matrix given below by a unique rotation (F ¼ RU and RRT ¼ I), and e^ is any direction in which the transformation strain is calculated.

More detailed explanations can be found in Saburi and Nenno [30], Sehitoglu et al. [34] and in a textbook by Bhattacharya [43]. The volumetric strain can be obtained as detðUÞ 1. This volumetric strain was used to estimate the transformation strain in the third dimension when in-plane strains were measured via DIC.

The entire stereographic triangle for the three alloys is given in Fig. 18 showing the maximum transformation strains. We calculated the Ni2FeGa and CuZnAl

transfor-mation strain stereographic triangles in this study while the NiTi stereographic triangle (the detwinning strain version) was published previously [43].

The important observation is that the transformation strains in all shape memory alloys considered are as high as 10 %. We point out that transformation strains were mea-sured for the Ni2FeGa at the maximum and minimum loads and were used in the calculations. Because we do not have the experimental results of DIC measurements during fa-tigue crack growth for NiTi and CuZnAl, these strains were assumed to be the same magnitude as Ni2FeGa. Admit-tedly, this is a considerable effort that needs to be under-taken in future studies.

### Appendix

### 5: Elastic Moduli Determination

An example of the energy variation as a function of the applied displacement fields is illustrated in Fig. 19 to establish the elastic constants in tetragonal Ni2FeGa.

In the following analysis, we demonstrate how to
cal-culate the C_{33 }for tetragonal Ni2FeGa. We applied small
strain (d) varying from -0.03 to 0.03 to minimize the
er-rors from higher order terms in the following equation:

Fig. 15 The principal equivalent eigenstrains for three materials (CuZnAl, NiTi and Ni2FeGa). The factor F is applied to NiTi and

CuZnAl indicating that the magnitude of the strains are smaller in those two materials

where k is C12, l is C44, l0is C11–C12–2C44, a1, a2, and a3
are the semi axis align with the coordinate x, y and z. For
the case of flat ellipsoid (a_{1 }[ a2 [ a3), q is assumed to be
infinity (Fig. 15).

### Appendix

### 2: The Weight Functions

Earlier, the calculation of weight function was introduced as the following.

E Vð ;eÞ ¼ E Vð o; 0Þ þ Vo
X6
i¼1
rieiþ
Vo
2
X6
i;j¼1
Cijeiejþ O e3
:
ð20Þ
The distortion matrix to calculate C_{33 }(see Table 2) is
given by

e3¼ d

Table 8 The transformation matrix components for Ni2FeGa, NiTi,

and CuZnAl Material U11 U22 U33 U12 U13 U23 Ni2FeGa 0.9354 0.9354 1.1354 0 0 0 NiTi 0.9563 1.0243 1.0243 -0.0427 -0.0427 0.0580 CuZnAl 1.0101 1.0866 0.9093 0.0249 0 0 Fig. 17 continued

Fig. 18 The transformation strains in tension for Ni2FeGa, NiTi and CuZnAl considered in this study

Therefore, Eq. (20) becomes E V;ð dÞ ¼ E Vð o; 0Þ þ Vo r3dþ C33 2 d 2 : ð21Þ

We calculate the energy variation of the crystal sub-jected to different magnitudes of strain and the results are shown in Fig. 19b. The blue curve is a second-order polynomial function to fit these values, and can be written as follows:

Eð Þ ¼ 62:87dd 2_{ 0:1006d 45:812:} _{ð22Þ}

We equate the second-order coefficient of Eq. (22) to the
C_{33 }elastic constant in Eq. (21) (note that the energy unit is
eV, and 1 eV = 1.6 9 10-19 J), and calculate the C_{33 }as
follows:
Vo
C33
2
d2 ¼ 62:87 1:6 10 19_{d}2 _{ð23Þ}

Substituting the volume of the crystal (Vo) to be 94.69 A˚ = 94.69 9 10-30 m3 into Eq. (23), we calculate

the C_{33 }to be 212 GPa. All other elastic constants are
calculated following similar procedure.

### References

1. Duerig TW, Melton K, Stockel D, Wayman C (1990) Engineer-ing aspects of shape memory alloys. Butterworth-Heinemann, London

2. Otsuka K, Wayman CM (eds) (1998) Shape memory materials. Cambridge University Press, Cambridge

3. McMeeking RM, Evans AG (1982) Mechanics of transformation-toughening in brittle materials. J Am Ceram Soc 65:242–246 4. Rice JR (1972) Some remarks on elastic crack-tip stress fields. Int

J Solids Struct 8:751–758. doi:10.1016/0020-7683(72)90040-6 5. Xiong F, Liu Y (2007) Effect of stress-induced martensitic

transformation on the crack tip stress-intensity factor in Ni-Mn-Ga shape memory alloy. Acta Mater 55:5621–5629. doi:10.1016/ j.actamat.2007.06.031

6. Irwin GR (1960) Plastic zone near a crack and fracture toughness. In: Proceedings of the Sagamore Res Ord Materials Section IV, pp 63–71

7. Baxevanis T, Parrinello AF, Lagoudas DC (2013) On the fracture toughness enhancement due to stress-induced phase transforma-tion in shape memory alloys. Int J Plast 50:158–169. doi:10.1016/ j.ijplas.2013.04.007

8. Lexcellent C, Thiebaud F (2008) Determination of the phase transformation zone at a crack tip in a shape memory alloy ex-hibiting asymmetry between tension and compression. Scripta Mater 59:321–323. doi:10.1016/j.scriptamat.2008.03.040 9. Stam G, van der Giessen E (1995) Effect of reversible phase

transformations on crack growth. Mech Mater 21:51–71. doi:10. 1016/0167-6636(94)00074-3

10. Brown LC (1979) The fatigue of pseudoelastic single crystals of a-CuAINi. Metall Mater Trans A 10:217–224. doi:10.1007/ BF02817631

11. Delaey L, Janssen J, Van de Mosselaer D, Dullenkopf G, Deruyttere A (1978) Fatigue properties of pseudoelastic

CuZnAl alloys. Scripta Metall. 12:373–376. doi:10.1016/0036-9748(78)90302-2

12. Hornbogen E, Eggeler G (2004) Surface aspects in fatigue of shape memory alloys (SMA). Mater. Werkst 35:255–259. doi:10. 1002/mawe.200400759

13. Melton KN, Mercier O (1979) Fatigue of NiTi thermoelastic martensites. Acta Metall 27:137–144

14. Miyazaki S, Mizukoshi K, Ueki T, Sakuma T, Liu Y (1999) Fatigue life of Ti–50 at.% Ni and Ti–40Ni–10Cu (at.%) shape memory alloy wires. In: ICOMAT 98. International conference on martensitic transformations, 7–11 Dec. 1998. Elsevier, pp 658–663. doi:10.1016/s0921-5093(99)00344-5

15. Sade M, Hornbogen E (1988) Fatigue of single- and polycrys-talline—CuZn-base shape memory alloys. Z Metall 79:782–787 16. Yang NYC, Laird C, Pope DP (1977) The cyclic stress–strain response of polycrystalline, pseudoelastic Cu-14.5 wt pct Al-3 wt pct Ni alloy. Metall Mater Trans A 8:955–962. doi:10.1007/ BF02661579

17. McKelvey AL, Ritchie RO (1999) Fatigue-crack propagation in Nitinol, ashape-memory and superelastic endovascular stent material. J Biomed Mater Res 47:301–308

18. McKelvey AL, Ritchie RO (2001) Fatigue-crack growth behavior in the superelastic and shape-memory alloy nitinol. Metall Mater Trans A 32:731–743. doi:10.1007/s11661-001-1008-7

19. Robertson SW, Mehta A, Pelton AR, Ritchie RO (2007) Evolu-tion of crack-tip transformation zones in superelastic nitinol subjected to in situ fatigue: a fracture mechanics and synchrotron X-ray microdiffraction analysis. Acta Mater 55:6198–6207 20. Holtz RL, Sadananda K, Imam MA (1996) Near-threshold fatigue

crack growth behavior of nickel-titanium shape memory alloys. In: Johannes Weertman symposium. Proceedings of a symposium held during the TMS annual meeting, 4–8 Feb. 1996, Warrendale, pp 297–299

21. Vaidyanathan R, Dunand DC, Ramamurty U (2000) Fatigue crack-growth in shape-memory NiTi and NiTi–TiC composites. Mater Sci Eng A 289:208–216. doi:10.1016/S0921-5093(00)00 882-0

22. Wang J, Sehitoglu H (2014) Martensite modulus dilemma in monoclinic NiTi-theory and experiments. Int J Plast 61:17–31. doi:10.1016/j.ijplas.2014.05.005

23. Hatcher N, Kontsevoi OY, Freeman AJ (2009) Role of elastic and shear stabilities in the martensitic transformation path of NiTi. Phys Rev B 80:144203

24. Wagner MFX, Windl W (2008) Lattice stability, elastic constants and macroscopic moduli of NiTi martensites from first principles. Acta Mater 56:6232

25. Eshelby JD (1957) The determination of the elastic field of an ellipsoidal inclusion, and related problems. Proc R Soc Lond Ser A Math Phys Sci 241:376–396. doi:10.2307/100095

26. Sih GC, Paris PC, Irwin GR (1965) On cracks in rectilinearly anisotropic bodies. Int J Fract Mech 1:189–203. doi:10.1007/ BF00186854

27. Efstathiou C, Sehitoglu H, Carroll J, Lambros J, Maier HJ (2008) Full-field strain evolution during intermartensitic transformations in single-crystal NiFeGa. Acta Mater 56:3791–3799. doi:10. 1016/ j.actamat.2008.04.033

28. Efstathiou C, Sehitoglu H, Lambros J (2010) Multiscale strain measurements of plastically deforming polycrystalline titanium: role of deformation heterogeneities. Int J Plast 26:93

29. Hamilton ARF, Sehitoglu H, Efstathiou C, Maier HJ (2007) Mechanical response of NiFeGa alloys containing second-phase particles. Scripta Mater 57:497–499

30. Saburi T, Nenno S (1981) The shape memory effect and related phenomena. In: Aaronson HI, Laughlin DE, Sekerka RF, Way-man CM (eds) International conference on solid-solid phase transformations, Pittsburgh, pp 1455–1479

31. Kresse G, Furthmuller J (1996) Efficient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Phys Rev B 54:11169

32. Rodriguez PL, Lovey FC, Guenin G, Pelegrina JL, Sade M, Morin M (1993) Elastic constants of the monoclinic 18R martensite of a CuZnAl alloy. Acta Metall Mater 41(11):3307–3310

33. Verlinden B, Suzuki T, Delaey L, Guenin G (1984) Third order elastic constants of b Cu-Zn-Al as a function of the temperature. Scripta Metall 18:975–979

34. Ranganathan SI, Ostoja-Starzewski M (2008) Universal elasti-canisotropy index. Phys Rev Lett 101(5):055504

35. Carroll J, Efstathiou C, Lambros J, Sehitoglu H, Hauber B, Spottswood S, Chona R (2009) Investigation of fatigue crack closure using multiscale image correlation experiments. Eng Fract Mech 76(15):2384–2398

36. Pe´rez-Landaza´bal JI, Recarte V, Sa´nchez-Alarcos V, Rodrı´guez-Velamaza´n JA, Jime´nez-Ruiz M, Link P, Cesari E, Chumlyakov YI (2009) Lattice dynamics and external magnetic-field effects in Ni-Fe-Ga alloys. Phys Rev B 80(14):144301

37. Ren X, Miura N, Zhang J, Otsuka K, Tanaka K, Koiwa M, Suzuki T, Chumlyakov YI, Asai M (2001) A comparative study of elastic

constants of Ti-Ni based alloys prior to martensitic transforma-tion. Mater Sci Eng A 312:196–206

38. Mura T (1987) Micromechanics of defects in solids, vol 3. Springer

39. Chowdhury PB, Sehitoglu H, Rateick RG (2014) Predicting fa-tigue resistance of nano-twinned materials: Part I—role of cyclic slip irreversibility and Peierls stress. Int J Fatigue 68:277–291 40. Chowdhury PB, Sehitoglu H, Rateick RG (2014) Predicting

fa-tigue resistance of nano-twinned materials: Part II—effective threshold stress intensity factor range. Int J Fatigue 68:292–301 41. Sehitoglu H, Wang J, Maier HJ (2012) Transformation and slip

behavior of Ni2FeGa. Int J Plast 39:61–74

42. Sehitoglu H, Zhang XY, Chumlyakov YI, Karaman I, Gall K, Maier HJ (2002) Observations on stress-induced transformations in NiTi alloys. In: IUTAM symposium on mechanics of martensitic phase transformation in solids. Springer, New York, pp 103–109

43. Sehitoglu H, Karaman I, Anderson R, Zhang X, Gall K, Maier HJ, Chumlyakov Y (2000) Compressive response of NiTi single crystals. Acta Mater 48(13):3311–3326